67551071 au-gold cementation with zinc powder at low cyanide
Journal of Applied Electrochemistry 30: 217±229, 2000. 217 Ó 2000 Kluwer Academic Publishers. Printed in the Netherlands.An electrochemical study of gold cementation with zinc powder at low cyanideconcentration in alkaline solutions ÂS. VILCHIS-CARBAJAL1, I. GONZALEZ2 and G.T. LAPIDUS1*1 Depto. de IngenierõÂa de Procesos e HidrauÂlica and2 Depto. de QuõÂmica, Universidad AutoÂnoma Metropolitana ± Iztapalapa, Av. La PurõÂsima y MichoacaÂn s/n, Apdo.Postal 55-534, Mexico, D.F. 09340, Mexico(*author for correspondence, e-mail: firstname.lastname@example.org)Received 19 January 1999; accepted in revised form 24 August 1999Key words: cementation, cyanide, Evans diagrams, gold, zinc powder passivationAbstractThe half-reactions involved in gold cementation on zinc powder from low concentration alkaline cyanide solutionswere studied in a steady state regime, employing electrodes of glassy carbon and graphite paste with zinc powder.The eects of pH, cyanide and initial gold concentrations were investigated using various electrochemical techniques.The results were used to determine the controlling step of the cementation at low cyanide concentration and tointerpret the in¯uence of the variables on this process. Mixed potentials and associated currents were determinedfrom the Evans diagrams constructed using sampled current±potentials curves from chronoamperometric results forhalf redox reactions. These values do not adequately describe the global cementation reaction because gold reductionin low cyanide concentration solutions is greatly in¯uenced by a strong contribution from adsorptive processes. Thisbehaviour is dierent from that found by other authors for concentrated gold and cyanide solutions, where theprocess is controlled by the complex ion diusion (Au(CN)À ). The strong component of adsorption found in the 2present work does not permit the determination, using the Evans diagrams, of the cementation velocity. Directmonitoring of the mixed potential was proposed, employing an electrode made of zinc powder in carbonpaste submerged in a gold cyanide solution. The results of these experiments at low cyanide concentrations showthat zinc oxidation is controlled by the formation of dierent passivating layers, the nature of which depended onthe pH of the solution, and that the gold reduction reaction is strongly in¯uenced by adsorption phenomena.1. Introduction Most authors have stated that the controlling step in the cementation is Au(CN)À ion transport to the zinc 2The extraction of gold from minerals and concentrates surface [4±9]. On the one hand, all authors employedwith cyanide is an important hydrometallurgical pro- high cyanide concentrations (P10À3 M CN)), which iscess, which has been studied for more than 100 years not common in industrial practice . On the other[1, 2]. Two of the most important steps in this process hand, Eisenmann proposed that the kinetics are domi-are gold leaching in an alkaline cyanide medium, nated ®rst by an adsorption equilibrium, followed byfollowed by its cementation with zinc powder, carbon electron transfer . This contradiction in the literatureadsorption or electrolysis. Generally, in industrial prac- constitutes another reason to study in more detail goldtice, where high concentrations of silver or copper are cementation at low cyanide concentrations.found, zinc cementation is preferred over the other two To clarify the passivation problem, an electrochemicalprocesses . study of gold cementation at low cyanide concentrations One of the most serious problems in the cementation (10)3 and 10)4 M) is proposed, which investigatesstage is the high cost of reagents. The reduction in individually each half reaction: gold reduction (cathodicconcentration of one of them, cyanide, results in an branch) and zinc oxidation (anodic branch) as proposedextremely negative consequence, zinc passivation. When by Ihsan et al. .this occurs, the controlling step of the process maychange and the amount of zinc powder must be Au(CN)À eÀ 3 Au0 2 CNÀ 2 1increased to raise the gold cementation to an acceptablelevel [4±6]. There is thus substantial motivation for Zn 2 OHÀ 3 Zn(OH)2 s 2 eÀ 2study of the cementation process under passivatingconditions . Zn(OH)2 4 CNÀ 3 Zn(CN)2À 2 OHÀ 4 3
218 Zinc oxidation passes through the intermediate prod- 0.01 M Na2SO4 and 10)3 M NaCN at pH 10 and 10)6uct of Zn(OH)2 , whose stability is more important at and 10)3 M (Au(CN)À ). Subsequently, the capacitance± 2low cyanide concentrations [4, 5]. The most common potential diagrams were traced at this frequency. Forprocedure is to construct Evans diagrams, superim- these studies, the same potentiostat was used coupledposing the anodic and cathodic polarization curves. The with a Solartron (model 1260) frequency responsecrossover point of these curves is thought to determine analyser (FRA). Mixed potentials were measured withthe mixed potential and current associated with the a millivoltameter (PM2525) controlled by a personalcementation process. Using these values, in most cases, computer. Solutions were prepared with analytical gradeit is possible to interpret the velocity and controlling step chemicals and deionized water. The electrolyte supportof the cementation [5, 7, 8]. consisted of 10)4 or 10)3 M sodium cyanide and 10)2 M Na2SO4 at pH 10 or 11. The solutions employed for gold reduction additionally contained 10)6 to 10)3 M2. Experimental methods Au(CN)À . These solution conditions were selected 2 because they represent actual values of industrial oper-Four electrochemical techniques were used: cyclic vol- ating parameters .tammetry, electrochemical impedance spectroscopy(EIS), chronoamperometry and direct mixed potentialmeasurement. All experiments were performed in a three 3. Results and discussionelectrode cell under a nitrogen atmosphere at a temper-ature of 30 °C. The electrode arrangement included a 3.1. Gold reductionsaturated sulfate electrode as reference (SSE), a graphitecounterelectrode and the working electrode, which was Figures 1 and 2 show the voltamperometric behaviourzinc powder in a carbon paste matrix for zinc oxidation of a glassy carbon electrode submerged in a solutionor a glassy carbon bar mounted in a Te¯on support for which contain only cyanide and sodium sulfate. Athe gold reduction studies. Usually, a gold electrode is saturated sulfate reference electrode (SSE, 0.616 V vsemployed to study gold reduction when Au(I) concen- NHE) was employed for the entire study which wastrations are high (>10)3 M), however with the low favoured over chloride since sulfate ion is always presentconcentrations used in the present investigation, the in mineral leach solutions, due to the coexistence ofcapacitative and reductive currents are of the same order metal sul®des. Figure 1 shows the behaviour of solu-of magnitude, camou¯aging the nature of the process. tions with ®xed cyanide concentrations (10)4 M, Fig-Also, since the quantities of gold deposited on the ure 1(a) and 10)3 M, Figure 1(b)) and variable pH (10electrode are small, the only way to con®rm that a and 11). Figure 2 shows the behaviour at ®xed pHreduction has taken place is studying the oxidation of values (pH 10, Figure 2(a) and pH 11, Figure 2(b)) withthe recently formed metal over a substrate of a different variable cyanide concentrations (10)4 M and 10)3 M).material, in this case a glassy carbon electrode (GCE). Although these two Figures show the same data, theThe carbon paste zinc electrode (Zn(CPE)) has the manner in which the information is combined allowsadvantage of maintaining the original geometry of the the appreciation of the differences and similarities. Thesolid species used in the cementation process and for potential scan commences at 0.5 V in the cathodicthat reason reproducibility is very high . The use of direction to )2.0 V (direct scan), then, at this potential,(Zn(CPE)) is even more bene®cial than suspended the scan is inverted ending in 0.5 V. In the direct scan, aparticles because it allows a detailed study of the wave is observed at approximately )1.0 V. Because itinterface. The zinc powder carbon paste prepared in could not correspond to a faradaic reduction of thethis study was completely homogeneous. An estimate of electrolytic medium, the wave can only be associated tothe surface area was made by evaluating the geometric the adsorption of cyanide. The corresponding current ofarea of the electrode (Zn(CPE)) in contact with the this wave is more important at pH 10 than at pH 11 forelectrolyte (3.14 ´ 10)2 cm2). the different concentrations of cyanide (Figure 1). This The perturbation signal (potential) and the response behaviour is probably due to the competition between(current against potential or current against time) were the cyanide and hydroxyl ions for adsorption sites onobtained using a EGG PARC potentiostat (model the GCE surface. Alternatively, it may be seen in273A) linked to a personal computer. Capacity mea- Figure 2 that, at the same pH, the in¯uence of thesurements of the glassy carbon cyanide solution inter- cyanide concentration on the adsorption wave is mini-face were performed in the following manner. Initially, mal, indicating saturation of the electrochemical mono-impedance diagrams at dierent imposed potentials layer.were generated in the interval 0.01 Hz to 10 kHz. From To con®rm the existence of a capacitative eect atthese, the frequency was selected where the interfacial the interface, an impedance study was undertaken at thecapacitative time constant was predominant: (a) 30 Hz same conditions. Figure 3 shows the variation of thefor interface (GCE)/solutions containing 0.01 M interfacial capacitance as a function of E (the imposedNa2SO4 and 10)3 M NaCN at pH 10 and 11 and (b) potential). The interfacial capacitance for pH 11 is lower10 Hz for the interface (GCE)/solutions containing over the whole potential range. The notable dierence
219Fig. 1. Typical voltammograms obtained on (GCE) at 50 mV sÀ1 in aqueous solution containing 0.01 M Na2SO4, at dierent pH: (ÐÐ) 10 and11 (- - - -). NaCN concentration was modi®ed: (a) 10À4 M and (b) 10À3 M.between the capacitance values at both pH indicates a peak. A faradaic reduction of gold exists (peak A),modi®cation of the ions adsorbed at the interface. which is evidenced during the reverse scan by the In Figure 4, the voltammograms of the supporting appearance of peak AH at )0.925 V, representative ofelectrolyte are compared to those of each solution gold oxidation (Figure 4(c)). This faradaic reductioncontaining gold (10)6, 10)5 and 10)3 M) at pH 10 and a provokes a modi®cation of the capacitance of thisconstant cyanide concentration (10)3 M). The medium interface (Figure 5(c)). In this case, the oxidation±adsorption (wave at )1.0 V) is less favourable as the reduction process may be represented by Equation 1.gold concentration increases. Another wave is observed The conditional potential associated with this system atat a potential of )1.8 V for gold concentrations of 10)5 the experimental conditions is )1.035 vs SSE . Theand 10)6 M, which is independent of the gold concen- difference between this value and that of peak AH istration (Figure 4 (a) and (b)). This fact and the shape of minimal and may be attributed to electrocrystallizationthe peaks suggest adsorption of the gold cyanide processes. Therefore, it may be con®rmed that thecomplex (Au(CN)À ). This hypothesis is con®rmed by 2 aforementioned peaks A and AH correspond to thethe reduction in interfacial capacitance when Au(CN)À 2 reduction±oxidation process of Au(CN)À .2is added to the solution containing 0.01 M Na2SO4 and When gold reduction occurs at high concentrations,10)3 M NaCN in different concentrations (Figure 5(a) water begins to be reduced on the recently formed gold,and (b)). When the gold concentration is greater camou¯aging the gold reduction peak (Figure 4(c)).(Figure 4(c)), the controlling step of the electrochemical Water reduction on glassy carbon usually takes place atprocess changes, modifying the characteristics of this more negative potentials; however, the presence of
220Fig. 2. Typical voltammograms obtained on (GCE) at 50 mV sÀ1 in aqueous solution containing 0.01 M Na2SO4, at dierent NaCNconcentration: (ÐÐ) 10À4 M and (- - - -) 10À3 M. pH was modi®ed: (a) 10 and (b) 11.metallic gold shifts the process toward more positive may be induced when the gold complex is adsorbed orpotentials. reduced at the surface, which would cause a large To dilucidate the in¯uence of the cyanide concentra- variation in the cathodic current when the gold complextion, the same study as shown in Figure 4 was carried concentration or the pH is modi®ed (Figures 6 and 7).out at a lower cyanide concentration (10)4 M) for the A chronoamperometric study was performed on goldgold cyanide concentrations of 10)6 and 10)3 M. The cyanide solutions to verify the presence of large adsorp-voltammograms of Figure 6 show that, even at the high tive eects which mask faradaic processes in thegold concentration (10)3 M) (Figure 6(b)), the adsorp- voltamperometric behaviour of the cyanide solutions.tive process of the gold cyanide complex is important. When cyclic voltammetry is employed, the energeticThe wide peak at )1.8 V still appears at this concentra- properties of the surface are modi®ed with time (depen-tion, indicating that for lower cyanide concentrations, dent upon the potential scan velocity), resulting in athe complex adsorption is greater. However, when the current where the contributions from the energeticpH is changed from 10 to 11 (Figure 7), the adsorptive changes and the associated reaction velocities areeffect of the gold complex is suppressed by the compet- combined. To separate the two types of contributions,ing hydroxyl ions. This contribution may be attributed chronoamperometry is used. To establish the voltam-to the small amount of free cyanide relative to the large perometric behaviour of gold reduction without thequantity of (Au(CN)À ). In these conditions, a modi®- 2 problems associated with cyclic voltammetry, I/E curvescation of the free cyanide concentration at the interface from the chronoamperograms were constructed.
221Fig. 3. Variation of the capacitance of the GCE/cyanide solution with the imposed potential. The capacitances were evaluated by (EIS) at 30 Hzat (GCE) immersed in an aqueous solution containing 10À3 M NaCN and 0.01 M Na2SO4 at dierent pH: (a) 10 and (b) 11. Figure 8 shows some of the typical I/E curves (Figure 8(b)). The selected sampling time for theseconstructed for a small sampling time (27 ms) for a curves allows observation preferentially of the capacitivelow gold concentration (10)6 M) and a constant cyanide contribution to the total current (this capacitive currentconcentration (10)3 M) at pH 10 (Figure 8(a)) and 11 is directly associated with adsorptive processes). TheFig. 4. Comparison between voltammograms obtained in (GCE) (50 mV sÀ1 ) electrolytic solution in the absence (ÐÐ) and in the presence of(Au(CN)À ) (- - - -). The electrolytic solution containing 10À3 M NaCN and 0.01 M Na2SO4 at pH 10. The concentration of (Au(CN)À ) was varied: 2 2(a) 10À6 M, (b) 10À5 M and (c) 10À3 M.
222Fig. 5. Variation of the capacitance of the GCE/cyanide solution with an imposed potential. The capacitances were evaluated by (EIS) at 10 Hzat the (GCE) immersed in an aqueous solution containing 10À3 M NaCN and 0.01 M Na2SO4 at pH 10 and dierent concentrations of(Au(CN)À ): (a) 0, (b) 10À6 M and (c) 10À3 M. 2associated current is greater at pH 11 (Figure 8(b)). The determined by monitoring the working electrode poten-same behavior was observed with larger sampling times tials starting from the time when the solution was ®rst(up to 5 s), however the response is ampli®ed at this introduced until the potential remained stable. The timeshort time. Since the Au(I) concentrations are identical for the system to reach this potential is called thein both solutions, this difference is indicative of a `solution conditioning time. The OCP at pH 10 ismodi®cation in the adsorptive processes. In Figure 9, )1.25 V, while the (OCP) for the solution at pH 11 isI/E curves for solutions with dierent concentrations of )0.6 V. Additionally, there exists a large dierence ingold (Figure 9(b) and (c)) and without gold (Fig- conditioning time (5 min at pH 10 and 15 min ature 9(a)) are shown at pH 10 and at a constant cyanide pH 11). This indicates that the cyanide solution interactsconcentration (10)4 M). If the current were due exclu- in a dierent manner with the zinc surfaces at the twosively to faradaic processes, this would be expected to pH values. Other authors [4, 5] have observed that atincrease with the gold concentration. However, the low cyanide concentrations a zinc hydroxide layer isassociated current actually decreases for the highest gold formed which should be of a dierent nature at pH 10concentration to a value lower than when there is no than at pH 11.gold present (supporting electrolyte). This indicates that Figure 10 shows typical voltammograms obtained onthe adsorptive effects are more important than the a graphite paste electrode containing zinc powderfaradaic ones. It may be concluded that the correspond- (Zn(CPE)) in aqueous cyanide media at pH 10 and 11.ing gold reduction current has an important contribu- The potential scans commence at the (OCP) andtion from adsorption processes that does not allow the proceed to 0.8 V (direct scan), at which point theexact determination, by these methods, of the faradaic potential scan is inverted and brought back to )2.0 Vcurrent that is associated with metallic gold formation. (reverse scan). In the direct scan (anodic), a largeThis behaviour is due to the low cyanide concentration, oxidation peak is observed (BH and B1H ), which may bewhich differs from the ®ndings of other authors [5, 7], associated with the formation of zinc hydroxides thatwho worked at high cyanide concentrations. passivate the metal surface [4, 5] due to the low cyanide concentration (Equations 2 and 3). When the potential3.2. Zinc oxidation is inverted, the formation of these hydroxides continues since an oxidation current still exists in the inverse scan.The behaviour of the (Zn(CPE)) was studied in solutions When the potential is more negative ()1.7 V), a smallcontaining 0.01 M Na2SO4 and 10)3 M NaCN at pH 10. peak appears which corresponds to the reduction of theThe presence of sulfates modi®es the oxidation±reduc- zinc that had been dissolved in the oxidation process.tion behaviour of zinc relative to that reported in This last statement is supported by the fact that saidsolutions containing only cyanide. However, because of peak disappears when the solution is agitated or whenthe very small quantity of cyanide employed, the use of a the potential scan is initiated in the opposite (cathodic)supporting electrolyte was necessary. direction. Finally, the process observed in the limit of In electrochemical studies that involve solid species it the cathodic scan is due to water reduction.is important to start from the open circuit potential The currents associated with the oxidation±reduction(OCP) to obtain reproducible results. The (OCP) was processes of zinc are greater at pH 11. However, to
223Fig. 6. Comparison between voltammograms obtained in (GCE) (50 mV sÀ1 ) electrolytic solution in the absence (ÐÐ) and in the presence of(Au(CN)À ) (- - - -). The electrolytic solution containing 10À4 M NaCN and 0.01 M Na2SO4 at pH 10. The concentration of (Au(CN)À ) was 2 2varied: (a) 10À6 M and (b) 10À3 M.obtain a large current for zinc dissolution at this pH, tion peaks (BH and B1H ) and is associated with themore positive potentials are required than those needed metallic zinc, recently formed in the reduction processat pH 10 (BH ) and (B1H ). The dierences in the current represented by peak C. The half potential E1a2magnitude and the potential of the oxidation peak Epc Epa a2 from peaks C and CH is )1.47 V vs SSE,(B1H ) obtained at pH 11 with respect to peak (BH ) at comparable to the conditional potential associated withpH 10, leads to the supposition that the surface of zinc this system (Zn(OH)2/Zn) at these experimental condi-hydroxide at the two pHs are dierent. The large tions ()1.622 V) , con®rming the hypothesis thatoxidation current in the inverse scan, more pronounced peaks C and CH correspond to the zinc oxidation±for pH 11 than for pH 10, indicates that the passive reduction system.layer of zinc hydroxide formed at pH 11 continues to It may be assumed that at this low bulk cyanidedissolve at more negative potentials, probably due to concentration and with the large rate of zinc dissolution,the higher concentration of hydroxyl ions. This hy- the interfacial cyanide may be limited. In this situation,pothesis is con®rmed by peak (C), much larger for the solubility of the super®cial zinc hydroxide is apH 11, which represents the reduction of soluble function of both the cyanide and the hydroxyl ionZn(II), recently oxidized in the direct potential scan. concentrations, as may be calculated from the complexWhen the scan is inverted at )2.0 V, peak CH is stability constants and the zinc hydroxide solubilityobtained, but only for pH 11. This peak appears at a product . Under these conditions, zinc hydroxideless negative potential ()1.05 V) than the other oxida- would be more soluble at pH 11 than at pH 10.
224Fig. 7. Typical voltammograms obtained on (GCE) at 50 mV sÀ1 in aqueous solution containing 10À3 M Au(CN)À , 10À4 M NaCN and 0.01 M 2Na2SO4, at dierent pH: (ÐÐ) 10 and (- - - -) 11. The potential and characteristics of peak CH are totally it is necessary to use the chronoamperometric techniquedierent from those observed for peaks BH and B1H . This performed in the potential range corresponding tocon®rms that the zinc powder employed in the carbon potentials less negative than that of the (OCP) (±0.8 topaste initially has a passive layer which requires an )1.25 V). In Figure 11, the I/E curves constructed atoverpotential to dissolve it, even at a high pH value. The dierent sampling times are shown for the oxidation ofcrossover potential of zinc oxidation and gold reduction (Zn(CPE)) in the supporting electrolyte at pH 10 andoccurs near the zinc (OCP). Since the objective of this 11. While the I/E curves obtained with cyclic voltamme-research is to study the cementation process, the try show very little dierence between the two pH valuesbehavior of the passive layer in this zone is required. near their (OCP)s, in the I/E curves, a sizeable In the voltammograms for pH 10 and 11 (Figure 10), dierence may be observed.no appreciable changes in oxidation current are ob- The currents associated with zinc oxidation at pH 11served near the (OCP) due to the limitations of this are more important than those at pH 10. In both cases,technique. To separate the contributions from the oscillations are observed which probably correspond toenergetic changes and the associated reaction velocities, oxidation±passivation processes. The associated cur-Fig. 8. Sampled current±potential constructed from potentiostatic current transients obtained on (GCE) in aqueous solution containing 10À6 MAu(CN)À , 10À3 M NaCN and 0.01 M Na2SO4, at dierent pH: (a) 10 and (b) 11. Current was sampled at 27 ms. 2
225Fig. 9. Sampled current±potential constructed from potentiostatic current transients obtained on (GCE) in aqueous solution contained 10À4 MNaCN and 0.01 M Na2SO4, at pH 10 at dierent (Au(CN)À ): (a) 0, (b) 10À6 M and (c) 10À3 M. Current was sampled at 27 ms. 2rents diminish as the sampling time increases, indicating pHs 10 and 11 are quite dierent, con®rming thethat the oxidation process is strongly aected by observations made in the voltammograms (Figure 10).diusion. These modi®cations with time are also noted From the previous discussion it is possible to explainat pH 10, however, they are not perceivable in the why, even at the (OCP), the (Zn(CPE)) potential isFigure due to the large dierence in magnitude between variable at more basic values of pH.the currents at pH 10 and 11. In the I/E curves ofFigure 11, the abrupt increments are related to zinc 3.3. Evans diagramsoxidation and the sharp decreases to passivation. AtpH 11 the magnitude of the oscillations become more The ultimate purpose of studying the anodic behavior ofimportant as the potential is less negative. For less basic zinc and the cathodic behavior of gold is to generatepH values the oscillations are minimal, denoting a more Evans diagrams to evaluate the potential and velocityconstant process. This behaviour indicates that the of cementation. For the case analysed here, suchnature and character of the passivating layers formed at diagrams were constructed employing the current±Fig. 10. Typical voltammograms (50 mV sÀ1 ) obtained for metallic zinc in CPE (Zn(CPE)) in aqueous solution containing 10À3 M NaCN and0.01 M Na2SO4, at dierent pH: (ÐÐ) 10 and (- - - -) 11. The scan was initiated from OCP ()1.25 V at pH 10 and )0.6 V at pH 11) to anodicdirection.
226Fig. 11. Sampled current±potential constructed from potentiostatic current transients obtained on metallic zinc in CPE (Zn(CPE)) in aqueoussolution containing 10À3 M NaCN and 0.01 M Na2SO4, at dierent values of pH: (a) curves at 10 and (b) curves at 11. Current was sampled atdierent times: (h) 27, (,) 54 and (´) 74 ms.potential (I/E) curves obtained from the series of centrations equal to or larger than 10À5 M, threechronoamperograms for each half-reaction. Figure 12 crossover points are found due to the oscillations causedshows a typical diagram generated in this work. The by the zinc oxidation±passivation process. The crossoverzone where the I/E curves cross de®nes the controlling potentials and currents are essentially the same for thestep (adsorption, charge transfer or diusion). The supporting electrolyte and for all the gold concentra-mixed potential is that where the velocities of the anodic tions. This suggests that the controlling step of theand cathodic reactions are equal, which signi®es that no cementation is zinc oxidation and not gold reduction.net current is present. The anodic or cathodic current in However, the crossover potentials at these conditionsthis point would correspond to the cementation velocity. are near the cyanide adsorption wave (Figure 1). Addi- Table 1 shows the crossover potentials and currents tionally, it was demonstrated that at pH 11 the cyanideobtained from the corresponding Evans diagrams at adsorption wave was suppressed and, consequently, thedierent conditions. At 10À3 M cyanide and gold con- mixed potential was shifted to more negative valuesFig. 12. Evans diagrams for the redox system (Zn/Au(CN)À ) for the gold cementation by zinc in an aqueous solution containing 10À3 M NaCN 2and 0.01 M Na2SO4 at pH 10. The I/E curves were constructed from the corresponding potentiostatic current transients and the current weresampled at 27 ms. The zinc oxidation (- - - -) was obtained from Zn(CPE) and the gold reduction curves were obtained at dierent concentrationsof (Au(CN)À ): (ÐÐ) 10À6 M and (± - ± -) 10À5 M. 2
227Table 1. Crossover potentials and currents obtained from the corre- (ORP) of the solution. The former measures the inter-sponding Evans diagrams in solutions containing 0.01 M Na2SO4 and facial potential where the cementation process takes10)3 M NaCN at pH 10, the zinc oxidation was obtained fromZn(CPE) and the gold reduction curves were obtained at different place, while the latter detects the redox properties of the(Au(CN)À ) concentrations* 2 cementation solution (the (ORP) of the solution is determined using a platinum electrode). The mixed(Au(CN)À )/M 2 E/mV I/lA potential may be measured with a solid zinc bar, however,0 (Sup. elect.) )909 )46 its super®cial characteristics are completely dierent from10)6 )909 )45 those of zinc powder used in the industrial process. In10)5 )858 )49 order to approximate those conditions, a carbon paste )887 )60 electrode with this powder (Zn(CPE)) was used. )906 )6310)4 )872 )46 The change in potential with respect to time was )878 )46 determined using the (Zn(CPE)) electrode in the pres- )908 )47 ence of dierent electrolytes with distinct pH values and10)3 )854 )60 concentrations of gold and cyanide. In Figure 13, the )859 )65 potential±time (E/t) curves are shown for the Au(CN)À / 2 )905 )67 Zn0 system at dierent gold concentrations in 0.01 M * The Evans diagrams were constructed from sampled I/E curves at Na2 SO4 and 10À4 M NaCN at pH 10. In Figure 14, thea sample time of 74 ms. corresponding curves are plotted for the same condi- tions as before, but with a higher cyanide concentration(Table 2). This con®rms that the adsorption camou¯- (10À3 M).ages the gold reduction process. For this reason, these At both cyanide concentrations (Figures 13(b) andpotential and currents do not describe the conditions of 14(b)), oscillations in the value of the mixed potentialthe cementation process since at the mixed (crossover) are observed at pH 11. These oscillations are largerpotential it is not possible to observe the faradaic when the cyanide concentration is low (Figure 13(b)).contribution of gold. These results differ from those Oscillations in the potential are indicative of an oxida-found by other authors who studied this system at tion±passivation process probably due to the ¯aking ofhigher cyanide concentrations, where gold reduction is the passive layer. The absence of oscillation in the (E/t)limited by diffusion [5, 7]. curves at pH 10 (Figures 13(a) and 14(a)) imply that It may be concluded that in processes where adsorption considerable ¯aking does not exist at this pH, corrob-takes on a predominant role (for example in systems such orating that the passive layer is more stable. The valuesas [Au(CN)À ]/Au0, [Ag + ethylamine]/glassy carbon) 2 of the mixed potential are more negative with respect to[14±16], evaluation of the cementation velocity and the those obtained at pH 11 for both cyanide concentra-controlling step by means of Evans diagrams is not reli- tions. This dierence between the mixed potentials at theable. Consequently, the results produced with the tech- two pHs suggests that a distinct phenomena may beniques employed do not allow the precise determination controlling the cementation process at each pH. Aof the cementation velocity. Because of this, the direct pH 11, the controlling step may probably be zincdetermination of the mixed potentials of the Au(CN)À / 2 oxidation±passivation.Zn0 system was necessary in order to clear up those The oscillations observed in the intensity±potentialpoints where the validity of Evans diagrams is limited. curves generated from the chronoamperometric study of (Zn(CPE)) in cyanide solution (Figure 11) (where the3.4 Mixed potential of (Au(CN)À )/Zn0 system 2 oxidation is provoked electrically) are similar to those observed in Figures 13 and 14, where zinc oxidation isThe mixed potential of the Au(CN)À /Zn0 system should 2 chemically induced by the cementation reaction.not be confused with the oxidation±reduction potential For both levels of cyanide, the mixed potential be- comes less negative as the gold concentration increasesTable 2. Crossover potentials and currents obtained from the corre- (Figures 13 and 14). These variations indicate that atsponding Evans diagrams in solutions containing 0.01 M Na2SO4 and pH 10 the controlling step is the gold reduction. This10)3 M NaCN at pH 11, the zinc oxidation was obtained from reduction is aected by the adsorptive processes ofZn(CPE) and the gold reduction curves were obtained at different(Au(CN)À ) concentrations* cyanide and of the gold cyanide complex, illustrated by 2 the dierence in the E/t behaviour when the cyanide(Au(CN)À )/M 2 E/mV I/lA concentration is modi®ed at the same gold concentra-0 (Sup. elect.) )1232 )101 tion and pH. )1269 )106 In this manner it can be shown that while the )1323 )111 adsorptive eects do not allow the obtention of infor-10)6 )1232 )104 mation on the gold reductive processes from the Evans )1271 )111 diagrams, the evaluation of the mixed potentials permit )1303 )116 the detection of variations in the cementation process * The Evans diagrams were constructed from sampled I/E curves at when the conditions are modi®ed. Figures 13 and 14a sample time of 74 ms. suggest that the cementation process presents optimum
228Fig. 13. Variation of the mixed potential of metallic zinc in CPE (Zn(CPE)) with the immersion time in aqueous solution containing 10À4 MNaCN and 0.01 M Na2SO4 at dierent concentrations of (Au(CN)À ) and pH: (a) 10À6 M at pH 10, (b) 10À6 M at pH 11 and (c) 10À3 M at pH 10. 2Fig. 14. Variation of the mixed potential of metallic zinc in CPE (Zn(CPE)) with the immersion time in aqueous solution containing 10À3 MNaCN and 0.01 M Na2SO4, at dierent concentrations of (Au(CN)À ) and pH: (a) 10À6 M at pH 10, (b) 10À6 M at pH 11 and (c) 10À3 M at pH 10. 2E/t curves for the Au(CN)À /Zn0 system at two gold concentrations (10À6 M and 10À3 M Au(CN)À ) at pH 10 and 10À4 M CNÀ . 2 2conditions at pH 10 and when the ratio of cyanide to Generally, it has been found that at high cyanidegold is large. concentrations, gold reduction is limited by a diusional process. However, at low cyanide concentrations, as those used in industrial practice, the present study4. Conclusions determined that gold reduction is in¯uenced by the competitive adsorption between the cyanide, hydroxylThe following may be concluded with respect to zinc and gold dicyanide ions. At high concentrations of goldpowder oxidation in cyanide solutions: initially the zinc in solution, cyanide is replaced by Au(CN)À on the 2powder is covered by a passive hydroxide coating which electrode surface. However, in more alkaline solutions,requires a large overpotential to dissolve. The charac- gold adsorption is suppressed by the competition ofteristics of this layer are dierent at two distinct values hydroxyl ions for the same sites. At pH 10 and lowof pH, being much more stable at pH 10 than at pH 11. cyanide concentration, the faradaic reduction of gold isAt the latter pH, an oxidation±passivation process was evident only when this is present at the highest concen-observed using chronoamperometric and mixed potential tration (10À3 M).measurement techniques. The formation and dissolution Because gold reduction is completely concealed by theof the hydroxide layer is strongly aected by the pH. strong adsorptive processes, the construction of Evans
229diagrams from chronoamperometric curves does not 2. E.M. Hamilton, `Manual of Cyanidation (McGraw-Hill, Newre¯ect the cementation process and consequently, the York, 1950). 3. M.C. Jha, in Proceedings of the First International Symposium onmixed potentials obtained may not be valid. This was `Precious Metals Recovery Reno, Nevada, 10±14 June 1984,con®rmed by the direct measurement of the mixed p. XXI-1.potentials. From these potentials it was possible to 4. B. Ihsan, B. Hermann and Y. Atila, Erzmetall 33 (1980) 399.conclude that the controlling step of the cementation 5. J.D. Miller, R.Y. Wan and J.R. Parga, `Precious and Rare Metalchanges when the pH is modi®ed from 10 to 11, where Technologies, edited by A.E. Torma and I.H. Gundiler (Elsevier, Amsterdam, 1989), p. 281.zinc oxidation determines the kinetics of the process. At 6. R.L. Paul and D. Howarth, Proceedings of the InternationalpH 10, the kinetics are aected by the competitive Conference of Gold. Extractive Metallurgy of Gold (SAIMM,adsorption between the gold dicyanide complex and Johannesburg, 1986), p. 156.the free cyanide ion. For this reason, a practical 7. M. Nicol, E. Schalch, P. Balestra and H. Hegedus, J. South Afr.suggestion to obtain an optimum cementation velocity Inst. Min. Met. 79 (1979) 191. 8. F. Lawson, in `Thermodynamics and Kinetics of Metallurgicalis to operate at a low pH value (pH 10) with a high Processes edited by M.M. Rao, K.P. Abraham, G.N.K. Iyengar,cyanide to gold ratio. and R.M. Mallya (The Indian Institute of Metals, Calcutta, 1985), p. 207. 9. N.A. Sareyed-Dim and F. Lawson, Trans. Inst. Min. Met. 85Acknowledgements (1976) C1. 10. E.T. Eisenmann, J. Electrochem. Soc. 125 (1978) 717.The authors wish to thank CONACyT (Mexican Na- Â Â 11. I. Lazaro, N. MartõÂ nez, I. RodrõÂ guez, E. Arce and I. Gonzalez,tional Science and Technology Foundation) for the Hydrometallurgy 38 (1995) 277. 12. A.J. Bard, R. Parsons and J. Jordan, `Standard Potentials inpostgraduate scholarship awarded to Soledad Vilchis- Aqueous Solution (Marcel Dekker, New York, 1985), p. 254.Carbajal. 13. A.E. Martell and R.M. Smith, `Critical Stability Constants Vols 4 and 6 (Plenum Press, New York, 1976 and 1982). 14. W. Chrzanowski, Y. Li and A. Lasia, J. Appl. Electrochem. 26References (1996) 385. 15. D.M. MacArthur, J. Electrochem. Soc. 119 (1972) 672.1. J. Dorr and F. Bosqui, `Cyanidation of Gold and Silver Ores Â Â 16. M. Miranda-Hernandez and I. Gonzalez, Electrochim. Acta 2 (McGraw-Hill, New York 1950), p. 184. (1997) 2295.